# Nonlinear Optical Phenomena and Materialsrlbyer/PDF_AllPubs/1974/32.pdfNONLINEAR OPTICAL PHENOMENA...

date post

20-Apr-2020Category

## Documents

view

5download

0

Embed Size (px)

### Transcript of Nonlinear Optical Phenomena and Materialsrlbyer/PDF_AllPubs/1974/32.pdfNONLINEAR OPTICAL PHENOMENA...

Copyright 1974. All rights reserved

NONLINEAR OPTICALPHENOMENA AND MATERIALS

~8554

Robert L. Byer

Department of Applied Physics, Stanford University, Stanford, California 94305

INTRODUCTION

The field of nonlinear optics has developed rapidly since its beginning in 1961. Thisdevelopment is in both the theory of nonlinear effects and the theory of nonlinearinteractions in solids, and in the applications of nonlinear devices. This reviewdiscusses nonlinear interactions in solids and the resultant nonlinear coupling ofelectromagnetic waves that leads to second harmonic generation, optical mixing, andoptical parametric oscillation. Material requirements for device applications areconsidered, and important nonlinear material properties summarized. At the outset,a brief review of the development of nonlinear optics and devices is in order to provideperspective of this rapidly growing field.

Historical Review

In 1961, shortly after the demonstration of the laser, Franken et al (1) generated thesecond harmonic of a Ruby laser in crystal quartz. The success of this experimentrelied directly on the enormous increase of power spectral brightness provided bya laser source compared to incoherent sources. Power densities greater than109 W/cm2 became available; these correspond to an electric field strength of106 V cm- 1. This field strength is comparable to atomic field strengths and, there-fore, it was not too surprising that materials responded in a nonlinear manner tothe applied fields.

The early work in nonlinear optics concentrated on second harmonic generation.Harmonic generation in the optical region is similar to the more familiar harmonicgeneration at radio frequencies, with one important exception. In the radio frequencyrange the wavelength is usually much larger than the harmonic generator, so thatthe interaction is localized in a volume much smaller than the dimensions of awavelength. In the optical region the situation is usually reversed and the nonlinearmedium extends over many wavelengths. This leads to the consideration of propa-gation effects since the electromagnetic wave interacts over an extended distancewith the generated nonlinear polarization. The situation is similar to a propagatingwave interacting with a phased linear dipole array. If this interaction is to be efficient,

147

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

148 BYER

the phase of the propagating wave and the generated polarization must be proper. Innonlinear optics this is referred to as phasematching. For second harmonic genera-tion, phasematching implies that the phase velocity of the fundamental and secondharmonic waves are equal in the nonlinear material. Since optical materials aredispersive, it is not possible to achieve equal phase velocities in isotropic materials.Shortly after Franken et al’s first relatively inefficient nonphasematched secondharmonic generation experiment, Kleinman (2), Giordmaine (3), and Maker et (4), and later Akhmanov et al (5) showed that phase velocity matching could achieved in birefringent crystals by using the crystal birefringence to offset thedispersion.

Along with the important concept of phasematching, other effects leading toefficient second harmonic generation were studied. These included focusing (6, 7),double refraction (8-10), and operation of second harmonic generators with external resonator (i 1, 12) and within a laser cavity (13, 14).

An important extension of nonlinear interactions occurred in 1965 when Wang& Racette (15) observed significant gain in a three-frequency mixing experiment. Thepossibility of optical parametric gain had been previously considered theoretically¯ by Kingston (16), Kroll (17), Akhmanov & Khokhlov (18), and Armstrong et al It remained for Giordmaine & Miller (20) in 1965 to achieve adequate parametricgain in LiNbO3 to overcome losses and reach threshold for coherent oscillation.This early work led to considerable activity in the study of parametric oscillatorsas tunable coherent light sources.

Simultaneously with the activity in nonlinear devices, the theory of nonlinearinteractions received increased attention. It was re.cognized quite early that progressin the field depended critically upon the availability of quality nonlinear materials.Initially, the number of phasematchable nonlinear crystals with accurately measurednonlinear coefficients was limited to a handful of previously known piezoelectric,ferroelectric, or electro-optic materials. An important step in the problem ofsearching for new nonlinear materials was made., when Miller (21) recognized thatthe nonlinear susceptibility was related to the third power of the linear susceptibilityby a factor now known as Miller’s delta. Whereas nonlinear coefficients of materialsspan over four orders of magnitude, Miller’s delta is constant to within 50~. Tothe crystal grower and nonlinear materials scientist, this simple rule allows theprediction of nonlinear coefficients based on known crystal indices of refraction andsymmetry, without having to carry out the expensive and time-consuming tasks ofcrystal growth, accurate measurement of the birefringence to predict phasematching,orientation, and finally second harmonic generation.

The early progress in nonlinear optics has been the subject of a number ofmonographs [Akhmanov & Khokhlov (22), Bloembergen (23), Butcher (24), Franken& Ward (25)] and review articles [Ovander (26), Bonch-Bruevich & Khodovoi(27), Minck et al (28), Pershan (28a), Akhmanov et al (29), Terhune & Maker Akhmanov & Khokhlov (31), and Kielich (32)]. hi addition, nonlinear materials been reviewed by Suvorov & Sonin (33), Rez (34), and Hulme (34a), compilation of nonlinear materials is provided by Singh (35). Two books haveappeared, one a brief introduction by Baldwin (36), and the second a clearly written

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 149

text by Zernike & Midwinter (37). Finally, a text covering all aspects of nonlinearoptics is to appear soon (38).

Nonlinear Devices

The primary application of nonlinear materials is the generation of new frequenciesnot available with existing laser sources. The variety of applications for nonlinearoptical devices is so large that I will touch only the highlights here.

Second harmonic generation (SHG) received early attention primarily because early theoretical understanding and its use for measuring and testing the nonlinearproperties of crystals. Efficient SHG has been demonstrated using a number ofmaterials and laser sources. In 1968 Geusic et al (39) obtained efficient doubling a continuous wave (cw) Nd : YAG laser using the crystal Ba2NaNbsO 1 s. That sameyear, Dowley (40) reported efficient SHG of an argon ion laser operating 0.5145/~m in ADP. Later Hagen et al (41) reported 70~ doubling efficiency of high energy Nd: glass laser in KDP (potassium dihydrogen phosphate), and Chesleret al (42) reported efficient SHG of a Q-switch Nd:YA(~ laser using LilOa. efficiently doubled Q-switched Nd : YAG laser is now available as a commercial lasersource (43). In addition, LiIOa has been used to efficiently double a Ruby laser (44).Recently the 10.6 pm CO2 laser has been dot~bled in Tellurium with .5~o efficiency(43) and in a ternary semiconductor CdGeAs~ with 15~ efficiency (46).

Three-frequency nonlinear interactions include sum generation, difference fre-quency generation or mixing, and parametric generation and oscillation. Aninteresting application of sum generation is infrared up-conversion and image up-conversion. For example, Smith & Mahr (47) report achieving a detector noiseequivalent power of 10-1, W at 3.5 pm by up-converting to 0.447 l*m in LiNbOausing an argon ion laser pump source. This detection method is being used forinfrared astronomy. Numerous workers have efficiently up-converted 10.6 #m to thevisible range (48-52) for detection by a photomultiplier. An extension of single beamup-conversion is image up-conversion (37, 53, 54). Resolution to 300 lines has beenachieved, but at a cost in up-conversion efficiency.

Combining two frequencies to generate the difl’erence frequency by mixing wasfirst demonstrated by Wang & Racette (15). Zernike & Berman (55) used approach to generate tunable far infrared radiation. Recently a number of workershave utilized mixing in proustite (36, 57), CdSe (58), ZnGeP2 (52, 52a), Ag(3aS2(59), and recently AgGaSe2 (60, 61) to generate tunable coherent infrared outputfrom near infrared or visible sources.

Perhaps the most unique aspect of nonlinear interactions is the generation ofcoherent continuously-tunable laser-like radiation by parametric oscillation in anonlinear crystal. Parametric oscillators were well known in the microwave region(62, 63) prior to their demonstration in the optical range. To date, parametricoscillators have been tuned across the visible and near infrared in KDP (29, 64,65) and ADP (66) when pumped at the second harmonic and fourth harmonic the 1.06 ~tm Nd : YAG laser, and they have been tuned over the infrared range from0.6 /~m to 3.7 #m in LiNbO3 (67-72). The above parametric oscillators werepumped by Q-switched, high peak power, laser sources. Parametric oscillators have

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

150 BYER

also been operated in a cw manner in Ba2NaNbsOl5 (73-76) and in LiNbO3 (77,78). However, the low gains inherent in cw pumping have held back research inthis area.

In 1969 Harris (79) reviewed the theory and devices aspects of parametricoscillators. Up to that time oscillation had been achieved in only three materials:KDP, LiNbO~, and Ba2NaNbsO~. Since 1969 parametric oscillation has beenextended to four new materials: ADP (80), LilO3 (8,1, 82), proustite (Ag3AsS3) (227),and CdSe (83). The new materials have extended the available tuning range. However,the development of oscillator devices still has remained materials limited. At this timeLiNbO3 is the only nonlinear crystal used in a commercially available parametricoscillatorJ Smith (84) and recently Byer (85) have discussed parametric oscillatorsin review papers and Byer (86) has reviewed their application to infrared spectroscopy.

Nonlinear interactions allow the extension of coherent radiation by secondharmonic generation, sum generation, and difference frequency mixing over a wave-length range from 2200/~ to beyond 1 mm in the far infrared, In addition, tunablecoherent radiation can be efficiently generated from a fixed frequency pump lasersource by parametric oscillation. The very wide spectral range and eff~ciency ofnonlinear interactions assures that they will become increasingly important ascoherent sources.

NONLINEAR PHENOMENA

Introduction

When a medium is subjected to an electric field the electrons in the medium arepolarized. For weak electric fields the polarization is linearly proportional to theapplied field

P = ~o)~lE

where Z1 is the linear optical susceptibility and % is the permittivity of free spacewith the value 8.85 x 10- ~2 F/m in inks units. The linear susceptibility is related to

the medium’s index of refraction n by ;El ~ n2_ 1.In a crystalline medium the linear susceptibility is a tensor that obeys the

symmetry properties of the crystal. Thus for isotropic media there is only one valueof the index, and for uniaxial crystals two values, no the ordinary and ne theextraordinary indices of refraction, and for biaxial crystals three values n~, n~, and

A linear polarizability is an approximation to the complete constitutive relationwhich can be written as an expansion in powers of the applied field, as

P = ~o[X~ +X2 "E+x3 "E2+...]E

where Z~ is the second order nonlinear susceptibility and )~3 is the third ordernonlinear susceptibility. A number of interesting optical phenomena arise from thesecond and third order susceptibilities. For example, )C" gives rise to second harmonic

a Chromatix Inc., Mountain View, California.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 151

generation (1), dc rectification (87), the linear electro-optic effect or Pockels effect(25), parametric oscillation (20), and three-frequency processes such as mixing and sum generation. The third order susceptibility is responsible for third harmonicgeneration (88), the quadratic electro-optic effect or Kerr effect (28), two-photonabsorption (89), and Raman (90), Brillouin (91), and Rayleigh (92) scattering.

We are primarily interested in effects that arise from Z2. For a review of thenonlinear susceptibility :Z2 and the resulting interactions in a nonlinear medium seeWemple & DiDomenico (93) and Ducuing & Flytzanis (93a).

To see how Z2 gives rise to second harmonic generation and other nonlineareffects, consider an applied field

E = E1 cos(klX-69t)+E 2 cos(k2x-o)t)

incident on the nonlinear medium. The nonlinear polarization is proportional toz2E2, giving

plus a similar term for frequency m2. This term describes both de r~tification andsecond harmonic generation. In addition, there are sum and mixing terms of the form

z2E~ E2[cos {(k~ - k2)x- (~, m2)t} +c os {( k~ + k~)x- (~ m2)t}

present in the expansion. These terms describe difference frequency and sumfrequency generation. All of the above processes take place simultaneously in thenonlinear medium. The question that naturally occurs is how one process is singledout to proceed efficiently relative to the competing processes. In nonlinear inter-actions phasematching selects the process of interest to the exclusion of the otherpossible processes. Thus, i~ the crystal birefringence is adjusted (by temperature orangle of propagation) such that second harmonic generation is the phasematchedprocess, then it proceeds with relatively high efficiency compared to the remainingprocesses involving sum and difference frequency generation.

CRYSTAL SYmmETrY Like the linear susceptibility, the second order nonlinearsusceptibility must display the symmetry properties of the crystal medium. Animmediate consequence of this fact is that in centrosymmetric media the secondorder nonlinear coefficients must vanish. Thus nonlinear optical effects are restrictedto acentric materials. This is the same symmetry requirement for the piezoelectric] tensors (94) and therefore the nonzero components of the second ordersusceptibility can be found by reference to the listed ] tensors. However, thenonlinear coefficient tensors have been listed in a number of references (24, 35, 37,95).

The tensor property of ~2 can be displayed by writing the nonlinear polarizationin the form

P~(oa) = eo ~ X~ E~(mz)E~(oO l.jk

where Zi~k(-- ma, ~o2, e)~) is the nonlinear susceptibility tensor.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

152 BYER

In addition to crystal symmetry restrictions, ;~i)~ satisfies two additional symmetry

relations. The first is an intrinsic symmetry relation which can be derived for alossless medium from general energy considerations (23, 96). This relation statesthat Zi~k(-- co3, c°2, c°1) is invariant under any permutation of the three pairs of indices(-c%, i); (co2,j); (col, k) as was first shown by Armstrong et al (19). The symmetry relation is based on a conjecture by Kleinman (2) that in a lossless mediumthe permutation of the frequencies is irrelevant and therefore ;(i~k is symmetri.c underany permutation of its indices.

Finally, it is customary to use reduced notation and to write the nonlinearsusceptibility in terms of a nonlinear coefficient di~g = di, n where m runs from 1-6with the correspondence

(jk)=(ll) (22) (33) (23) m= 1 2 3 4 5 6

and6

Pi(O)3)-----gO 2dir,(EE)r, 2.m=l

The 3 x 6 di~ matrix operates on the column vector (EE)r, given by2. 2.(EE)~ = E2~; (EE)2 = (EE) 3=Ez,

(EE),, = rEz; (E E)5=2ExEz; (E E)6 = xErAs an example, the nonlinear ~1 tensor for the 7~2rn point group to which KDP

and the chalcopyrite semiconductor crystals belong has the components

Px = 2dt,*ErEz; Pr = 2dta, ExEz; Pz =: 2d36ExEr 3.

However, Kleinman’s symmetry conjecture states that d~,~ = d~ equals d~6 =d~a~ since any permutation of indices is allowed. This is experimentally verified.Equation 1 and 2 show that

Zim( -- 093’ 0)1’ 092) 2dira( -- 0)3" 0)1, 0)2 4,

This defines the relation between the nonlinear susceptibility and the ~1 coefficientused to describe second harmonic generation. The definition of the nonlinearsusceptibility has been discussed in detail by Boyd & Kleinman (97) and Bechmann & Kurtz (95).

MILLER’S RULE We have not yet made an estimate of the magnitude of the nonlinearsusceptibility. An important step in estimating the magnitude of il was taken byMiller (21) when he proposed that the field could be written in terms of thepolarization as

E( - (.%) = 1__~ 2Ai~k(_ C03, cot, o)2)p.i(ot)e~(a)2) 5.80 jk

Comparing Equations 5 and 2 shows that the tensor ~l and A are related by

dijk = eO ~ Zil(f.o3)Z.im(0)2))(,kn(fol)Atran(--C93, 0)2, 0)1) 6.Iron

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 153

where glj = (n~- l) relates the linear susceptibility to the index of refraction. Millernoted that A is remarkably constant for nonlinear materials even though ~1 variesover four orders of magnitude.

Some insight into the physical significance of A can be gained by considering asimple anharmonic oscillator model representation of a crystal similar to the Drude-Lorentz model for valence electrons. This model has been previously discussed byLax et al (98), Bloembergen (23), Garrett & Robinson (99), and Kurtz & Robinson(100). For simplicity we neglect the tensor character of the nonlinear effect andconsider a scalar model. The anharmonic oscillator satisfies an equation

£+F~+~ooEx+~x2 = _e E(a), m

where F is a damping constant, ~ is the resonant frequency in the harmonicapproximation, and ~ is the anharmonic force constant. Here E(~, t) is consideredto be the local field in the medium. The linear approximation to the above equationhas the well known solution

Z(~) z- 1z z 2= = ~/(~0- ~ - iF~)2 -- Ne2/m% is the plasma frequency. Substituting th~ linear solution backwhere wp

into the anharmonic oscillator equation and solving for the nonlinear coefficient din terms of the linear susceptibilities gives

Ne3~ 1d=

60 m2 D(~I)D(~E)D(~3)

where D(~) is the resonant denomina.tor term in the linear susceptibility. Finally,using the relation between A and d given by Equation 6 we find that

[ m~o~A = ~NEea/ 7.

On physical grounds we expect that the linear and nonlinear restoring forces areroughly equal when the displacement x is on the order of the internuclear distancea, or when w~a ~ ~a2. In addition, if we make the approximation that Naa ~ 1 theexpression for A simplifies to

A = aE/e 8.

For a = 2 A the value for Miller’s delta predicted by our simple model is 0.25 m2/C.This compares very well with the mean value of 0.45 ~ 0.07 m2/C given by Bechmann& Kurtz (95).

Equation 6 shows that the second order susceptibility to a good approximationis given by

d ~ eoZ(C~)a)Z(C~)E)Z(c~h)A

~ eo(n2- 1)3A ~ eon6A

In nonlinear processes d2/na is the material nonlinear figure of merit. Figure 1 showsthis figure of merit and the transparvncy range for a number of nonlinear materials.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

154 BYER

I0,000

I000

I00

I0

0.10

0,01

z CdGeAs2

GaAsZnGePz

AgGaSe2TIzAsSe3

CdSe

I I I I I I I I~ ZO I0 5 2 I 0.5 0.2

TRANSI~RENCY RANGE (/~m)

Li ~03

Li 103

ADP

SiOz

Figure I Figure of merit and transparency range: for selected nonlinear crystals.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 155

Although dZ/n3 varies over four- orders of magnitude, the intuitive physical pictureinherent in the anharmonic oscillator model gives a remarkably accurate accountof the magnitude of a material’s nonlinear response.

Tt-IEORETICAL MODELS Although the anharmonic oscillator model gives insight intothe origin of the nonlinear susceptibility, it does not account for the tensor characterof ] or allow the calculation of the nonlinear force constant a.

The theory of the nonlinear susceptibility has been the subject of increasedconsideration. Historically, a quantum treatment based on a perturbation expansionof the susceptibility was the first description put forth for the nonlinear susceptibility(19, 23, 24, 101-104). Unfortunately, in solids, approximations to the quantum resultare required to obtain numerical results. In gases, where the wavefunctions arebetter known, the quantum expressions for the third order susceptibility (secondorder processes are not allowed by symmetry) do allow predictions of the magnitudeof Z3 which agree very well with measured values (105).

Robinson (106) was the first to attempt to simplify the complete quantumexpression for the nonlinear susceptibility. He approached the problem by lettingthe octapole moment of the ground state charge density serve as the eccentricityof the electronic cloud. Flytzanis & Ducuing (107, 108) and Jha & Bloembergen(109) applied this approach to the III-V compounds.

In the late 1960s Phillips & Van Vechten developed a theory for the dielectricproperties of tetrahedrally coordinated compounds (110, 111). This theory, based Penn’s (112) earlier theory of the dielectric susceptibility, is the basis for severalmodels describing the nonlinear susceptibility of crystals (107, 110, 113-119).

Briefly, the theory is based on a single energy gap description of the materialwhich is related to the dielectric constant by

e(0)- 2 2= ~p/E02 hNe2/m% is the plasma energy of the valence (ground state) electrons.where f~ =

Phillips & Van Vechten (110) have shown that the average energy gap Eo can bedecomposed into a covalent and ionic part Es and C by the relation E~2 = Es2 + Cz,

and that the ionicity of the bond is described by f~ = C2/E~. For the ionic orantisymmetric part of the bond, Phillips & Van Vechten (110) have shown that is described well by

where b is a constant, Z,~ and Z~ are the valence of elements A and B which formthe bond, and k~ is the Thomas-Fermi screening constant.

There are two approaches to calculating the nonlinear susceptibility based on theabove theory. The first is to interpret the theory as a two-band model and evaluatethe matrix elements appearing in the expansion for the second order susceptibility.This approach has been taken by Flytzanis (107), Phillips & Van Vechten (110),

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

156 BYER

and Kleinman (ll6). Using the method, Kleinman shows that the nonlinearcoefficient for zincblende compounds is

2

d,4=0.245~[ "a’~IC [" e2

where ao is the Bohr radius and Z is the linear susceptibility. The values of d~4predicted by Equation 9 are in good agreement wi~h experiment.

The second approach (113, 114) calculates the nonlinear susceptibility fromvariations in the linear susceptibility under an applied field. In this approach theposition of the bond charge can vary (the bond charge model) (113, 120) or a transferof charge along the bond axis can occur (the charge transfer model) (118, 119). approaches give good descriptions of the second order susceptibility. The extensionto the third order nonlinear coefficient has been considered recently by Chemla etal (121).

Levine (115) has modified and extended the bond charge model of Phillips Van Vechten (110). In summary, the bond charge theory does accurately accountfor both the magnitude and the si~ of the nonlinear susceptibility of most nonlinearmaterials. However, for the purpose of searching for new nonlinear materials orestimating the nonlinear coefficient of a potential nonlinear material, Miller’s rule isfar simpler to apply.

Second Harmonic Generation

We are now in a position to evaluate the nonlinear interaction in a crystal and tocalculate the conversion efficiency and its dependence on phase~natching andfocusing. Conceptually, it is easier to treat the special case of second harmonicgeneration and then to extend the principal results to three-frequency interactions.

The starting point for the analysis is Maxwell’s equations from which the travelingwave equation is derived in the usual manner. The traveling equation

V~E- ~oa~- ~ = ~o~ 10.

describes the electric field in the medium with a linear dielectric constant ~ drivenby the nonlinear driving polarization O2p/&~. It is customary to define the fieldsby the Fourier relations

E(r, t) = ~[E(r, o) exp {i(k" ot)} + c .c.]

and-

P(r, t) = kiP(r, o) exp {i(k" or)) + c .c

Substituting into Equation 10 making the usual slowly varying amplitude approxi-mations that o~P ~ ~oP ~ ~, k OE/& ~ O~E/Oz~, and ~E ~ E, and letting ~ = ~g~cbe the electric field loss per length, gives

1 ~E _ i~ocoP~ + eE + c & 2

for the equation relating the envelope quantities of the fields. Neglecting loss,

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 157

assuming a steady state solution, and using the definition given by Equation 3 forthe driving polarization, the above equation reduces to a pair of coupled nonlinearequations for the fundamental and second harmonic waves

dE(09)- i~E(2r~)E*ffo) exp(iAkz) 1 la.

dz

dE(2~0)dz - i~:E(~)E(09) exp (- 1lb.

where ~ = ~d/nc and Ak = k(2~)-2k(~) is the wavevector mismatch. At phase-matching Ak = 0 and n(~) = n(2~) since 2~n/2 where n isthe indexof refraction.Here we have introduced the interaction constant ~ which includes the nonlinearcoe~cient d.

The above coupled equations for second harmonic generation have beensolved exactly (19). It is useful to discuss the solution for second harmonic generationsince the results can be extended to three-frequency interactions. We proceed byconsidering the low conversion e~ciency case for a nonzero Ak, and then the highconversion e~dency case.

In the low conversion limit, the fundamental wave is constant with distance.Therefore, we set dE(~)/dz = 0 and integrate Equation 1

~~(z ~ ~)~1/2

dE(2~) i~E2(~) exp (- iAkz) gO g-l/2

which gives

E(2o9) [~_, = i~E2 (~) [exp (iAkl/2)- exp (iAkl/2)]- iAk

-2, ,, sin(Akl/2)= ~r~ ~099t ~

If we denote (sin x)/x by sinc x, note that the intensity is given by

/~/C~0I = ~-let2

then in the low conversion limit, the conversion efficiency is

I(2g°) -- 1~2/2 sine2 (~)

where

r:l:. = IE(09)I_ 2092

12.

13.n3¢3£o

This example shows that phasematching enters into the nonlinear conversionprocess through the phase synchronism 2factor sinc (Akl/2) which is unity at Akl = O.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

158 BYER

Also, the second harmonic conversion efficiency is proportional to Idl 2 and I ~, asexpected, and varies as the fundamental intensity. The above result holds in theplane wave focusing limit where I = P/A and the area A = nW~o/2 with Wo thegaussian beam electric field radius.

For high conversion efficiencies, Equations lla and llb can be solved byinvoking energy conservation such that E2(co)+E2(2co)--EiZnc where Einc is incident electric field at z ~ 0. The solution for perfect phasematching is the wellknown result

I(2co) _ tanh2 (~Ei,c z)

1(co)which for small ~:Eincz reduces to the low conversion efficiency result. In theory,second harmonic generation should approa6h 100~o as a tanh2x function. Inpractice, conversion efficiencies of 40-50~ are reached under optimum focusingconditions.

The solutions for second harmonic generation suggest that phasematching andfocusing are important if maximum conversion efficiency is to be achieved. Theimportant aspects of phasematching and focusing are discussed next.

PHASEMATCHING It immediately follows from Equation t2 that for second har-monic generation to be efficient, Ak must be zero. As stated earlier, this isaccomplished in birefringent crystals by utilizing the birefringence to overcome thecrystal dispersion between the fundamental and second harmonic waves. As aspecific example, consider phasematching in the negative (ne < no) uniaxial crystalKDP.

For a beam propagating at an angle 0m to the crystal optic axis, the extraordinaryinde~ is given by

[ 1 ]2 coS20m sin2Or"

where no and n~ are the ordinary and extraordinary indices of refraction at thewavelength of interest. Two types of phasematching are possible for negative uniaxialKDP :

Type I n2eW.(Om)Type II n~,o(Or") = ~[,,~ (Or.) + ~o

For positive uniaxial crystals (n~ > no) the extraordinary and ordinary indices arereversed in the Type I and II phasematching expressions (35).

Type I phasematching uses the full birefringence to offset dispersion and TypeII phasematching averages the birefringence to use’. effectively half of it in offsettingthe dispersion. A more important factor in choosing the type of phasematchingto be used is the nonlinear coefficient tensor. It must be evaluated to see that theeffective nonlinear coefficient remains nonzero. Thus for KDP where the 712m non-linear tensor has components given by Equation 3, Type I phasematehing requiresthat the second harmonic wave be extraordinary or polarized along the crystallo-graphic z axis. To generate this polarization, the fundamental waves ~nust be

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 159

polarized in the Ex and Ey direction arid thus be.ordinary waves. In addition, theproduct ExEr should be maximized. Therefore, the propagation direction in thecrystal should be in the (110) plane at 0m to the crystal optic or z axis. For thiscase, the effective nonlinear coefficient becomes deff= d sin 0,, and it is this coefficientthat is used in the SHG conversion efficiency expression. The effective nonlinearcoefficients for other crystal point groups have been calculated and listed (37, 97).In addition, the phasematching angles for a number of nonlinear crystals andpump lasers have been listed by Kurtz (1.22).

The above discussion for uniaxial crystals can be extended to biaxial crystals.As one might expect, the generalization becomes complicated. However, Hobden(123) has given a complete description of the process including a careful definitionof the three principle indices n~, n~, and n~.

One other aspect of phasematching is important in limiting SHG conversionefficiency. As the extraordinary wave propagates in the crystal, its power flowdirection differs by the double refraction angle p from its phase velocity direction.This walk-off of energy at the doubled refraction angle leads to a decrease inSHG efficiency due to the separation of the ordinary fundamental wave and theextraordinary second harmonic wave. The double refraction angle is given by

p ~ tan p = n~z(2m) no2(~o~) sin 20,.

Note that p = 0 at 0 = 0 and 0 = ~/2. The latter angle corresponds to a propagationdirection 90° to the crystal optic axis. Phasematching in this direction is referred toa 90° phasematching and has the advantage of not inducing Poynting vector walk-off.As shown in the next section, when p :# 0, the effective interaction length in thecrystal may be considerably reduced, thus reducing the conversion efficiency.Therefore, 90° phasematching is desirable when possible.

FOCUSING Up to this point we have assumed that the interacting waves are planewaves of infinite extent. In fact, the beams are usually focused into the nonlinearcrystal to maximize the intensity and interaction length. In addition, the waves areusually generated by laser sources and thus have a Gaussian amplitude profile withelectric field radius w. Gaussian beam propagation theory and laser resonators havebeen treated by a number of authors and will not be considered here. For thepresent discussion, the important factors of interest are (a) the form of the Gaussianbeam

E = Eo exp(- rZ/w2)

(b) the relation between the peak power and intensity

and (c) twice the distance over which the beam area doubles

2~n 2b = kw2 = ~-w

which is called the confocal distance.

14.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

160 BYER

TO include focusing, the SHG efficiency can be written in the form

I(co) - \rcn~0 n2~o c0c3: Eo lko h(B, ¢)15.

where I is the crystal length, k~ the wavevector in the crystal at the fundamentalfrequency, and h(B, ~) is the Boyd & Kleinman (97) focusing factor. The focusingfactor h(B, ~) is a functioffof the double refraction parameter

and the focusing parameter

where b is the confocal distance given by Equation 14.In general, h(B, ~) is an integral expression involving B and ~. However, it

reduces to simplified expressions in the proper limits. If we introduce the aperturelength 1, given by

and an effective focal length ly given by

If -- 7~W2k -- 2 b2

then the second harmonic conversion efficiency takes the limiting forms

It for (Ia, 1: >> l)

ll a for (lf>>l>>la)I(2co__~) KP,~. I: I,for (l

I(co) - 241.~ for (l~>la>>l:)4.75/} for (la>>l>>lf)

The first limit corresponds to the plane wave focusing case where h(~, B) ~ lib.This case holds until lib ~ 1, which is called the eonfocal focusing limit. The secondharmonic conversion efficient is optimum at lib = 2.84 where h(2.84, 0) = 1.06 (97).

If p ~a 0, then the aperture length may limit the interaction length to the secondand third cases. In practice, even a small walk-off angle may reduce the secondharmonic efficie/acy by 30 times for a given crystal length and focusing. It is there-fore very desirable to adjust the crystal indices of refraction to achieve 90° phase-matching if possible, In general, the last three of the above limits are not encounteredexperimentally. This discussion on focusing is intended to serve as a general intro-duction. A more detailed presentation is given by Boyd & Kleinman (97).

Three-Frequency Interactions

Three-frequency interactions include sum generation and difference frequencygeneration or mixing in which two waves are incident on the nonlinear crystal and

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 161

interact to generate a third wave, and parametric generation in which a high powerpump frequency interacts in a nonlinear crystal to generate two tunable frequencies.

We denote the three frequencies by (oI, ~o2, and ~o3 such that (o3 = (DE"~(D 1 isthe energy conservation condition and k3 = k2+ki+Ak is the momentum con-servation condition with Ak the momentum mismatch.

If we consider LiNbO3 as an example, the generated polarization now has threecomponents given by

P(o)I) = eo2d31E(~°3)E*(°~2)

P(c°2) = eo2d31E(°93)E*(col)P(~o3) eo2d3 ~ E(~o2)E(09x)

Substituting the polarization and electric field expressions at ~o~, co2, and o)3 intothe wave equation given by Equation 10 gives three coupled equations similar tothe two coupled equations previously derived for the SHG case :

dE1dz ~- cqE1 = tclE3E~exp(iAkz)

16a.

dE2d~- + ~2Ez = it~2E3E~’ exp(iAkz) 16b.

dE3d-~- + ~3 E3 = it¢3 E1 E2 exp (- iAkz) 16c.

where E(~oa) is now written El, ~:i = ~oi d/ni c, and ~i is the loss.We next investigate the solution of the above coupled equations for the three

frequency processes of interest. The coupled equations have been solved exactly(19, 124); however, we ~onsider only the simplified case of interacting plane wavesand weak interactions such that the pump wave is not depleted.

SUM GENERATION (UP-CONVERSION) For the case of sum generation ~o~ is a weakinfrared wave that sums with a strong pump wave at 092 to generate a high frequency(visible) wave at (03. Negligible pump depletion implies that dEz/dz = 0 so that three coupled equations reduce to a pair of Equations (16a and 16c). If we assumeno loss, Ak = 0, and a solution of the form erz with input boundary conditions thatE3(z = 0) = 0 and Ea(z = 0) = E~(0), the solution of the coupled equations

Ex(z) = El(0) cos

=X/~3 Et(0) sin E3(z)

where

Thus sum generation has an oscillatory solution with no net gain and a 100~oconversion for Fz = n/2. In the low conversion limit, sin Fz ~ Fz so that the up-conversion efficiency becomes

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

162 r~V~R

I~ _ (~o3/F2/2 sinc2 17.11(0)

where F2l2 --(2~o~o3d21212)/(nln2n3c3%) is equal to the previously derived conversion eNciency factor given by Equation 13. In the low conversion e~ciencylimit the sum generation e~ciency ~uals the SHG e~ciency as one expects fromphysical arguments. However, at high conversion e~ciencies the sum generationconversion oscillates while the SHG conversion approaches 1~ as tanh~ Fz.

Sum generation has been used to generate new frequencies in the same way asSHG. For example, 10.6 gm has been summed with 5.3 gm in CdGeAsa (125) generate the third harmonic of 10.6 ~ at 3.5 ~m. :Similar summing has been usedto generate the third harmonic frequency of a 1.~36 ~m Nd:YAG laser in KDPwith 60~ e~ciency (126).

Sum generation also allows infrared waves to be up-converted to the visible fordetection by a photomultiplier. Infrared up-conversion has been extensively studied(127-129) and applied to astronomical uses (47).

DIFFERENCE FREQUENCY GEN~ATION. For difference frequency generation or mix-ing the pump is the high frequency field at ~3. Therefore, lack of pump depletionimplies dE3/dz = 0 so that the coupled equations reduce to Equations 16a and 16b.Again assuming a solution of the form er~ and boundary conditions that E~(z = 0) E~(0) and Ez(0) = 0 results in the solution

E~(z) = E~(0) cosh

~(~) = ~(0) sinh Fz

Now we notice that exponential functions have replaced the sin and cos functionswhich occurred in the sum generation case. This implies that both the input fieldat ~ and the generated difference field at ~z grow during the nonlinear interactionat the expense of the pump field. Again in the limit of low conversion efficiencywhere sinh FI ~ Fl the mixing efficiency becomes

where F~l~ = (2m~m~dZl~I~)/(n~n~n~c~o) is the conversion eNciency which ~uals’ the SHG and sum generation e~ciency. However, now both waves grow and have

net gain. This suggests the possibility of parametric oscillation once the gainexceeds the losses.

Difference frequency generation or mixing has been used to measure parametricgain (130) and to generate new frequencies. Of particular interest is the generationof infrared and far infrared radiation by mixing in nonlinear crystals. A numberexperiments have recently been carried out using visible dye laser sources (56, 57)and near infrared sources (59, 61) to generate tunable infrared output.

PARAMETRIC GgNERATION For this case we assume a strong pump wave at ~ andequal input fields at ~ and ~. Again the three coupled equations reduce to

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 163

Equations 16a and 16b in the absence of pump depletion. The remaining pair ofequations are the same as for mixing; however, now the boundary conditions thatEl(z -- 0) -- El(0) and E2(z z 0) = E2(0) are inputs into the system. In fact, the inputfields need be only the quantum noise field associated with the gain of the parametricamplifier.

The general solution of Equations 16a and 16b for the above boundary conditionshas been given by Harris (79) and by Byer (85) in their review articles on parametricoscillators and is too long to reproduce here. However, for a single frequencyincident on a parametric amplifier, the gain defined by G2(/) I12( II2/IE2/01121- 1simplifies to

G2(/) ---- [’2/2 sinh2 ~]l 19..ol

where F2/2 ~ (2colCOEd21Ela)/(nln2n3C3eo) and g = [FE-(Ak/2)2]~. In the low gainlimit Equation 19 reduces to

G2(l) = F212 sinc2 (~/)

which shows that the parametric gain equals the SHG conversion efficiency in thislimit. In the high gain limit Equation 19 reduces to

G2(l) = (1/4) exp(2F/) for Ak/2 ~ g. In practice high gains have been reported (65, 86, 131) such that super-radiant operation is possible (126, 132).

Parametric amplifiers, like all linear amplifiers, have inherent noise. Since theparametric frequencies can be in the visible range and are on the order of 10- lo Wper watt of pump power, the noise emission is intense enough to be easily visibleas parametric fluorescence (133, 134). A striking color photograph of parametricfluorescence generated in LiNbO3 (135) is reproduced in a review article Giordmaine (136). Parametric noise emission can be considered generated by theamplified zero point fluctuations of the electromagnetic field (137-139). It can shown that the fluorescence noise power is given simply by Pnoise = (energy perphoton) x gain x bandwidth or approximately by Fnoise z hO) × [.2/2 X (c/2Anl) whereAn is the crystal birefringence and I the crystal length. For LiNbO3 the emittednoise power per watt is approximately 10-10 W, or one order of magnitude largerthan the spontaneous Raman scattering power. The noise power can be used tomeasure the gain, bandwidth, and tuning characteristics of a parameter oscillator priorto ever achieving threshold (133, 134). Parametric fluorescence also provides a veryaccurate method of measuring the nonlinear coefficient of a crystal since only a powerratio need be measured and not an absolute power as for SHG measurements (137).However, one of the most interesting applications of parametric generation is theachievement of coherent tunable laser-like output from an optical parametricoscillator.

Parametric Oscillators

A parametric oscillator is schematically represented by a nonlinear crystal withinan optical cavity. The nonlinear crystal when pumped provides gain at the two

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

164 BYER

frequencies 12o2 and 81 (the signal and idler fields). When the gain exceeds the lossthe device reaches threshold and oscillates. At threshold the output power increasesdramatically, similar to the behavior of a laser. The generated output is coherent andcollinear with the pump laser beam. Once above threshold, the parametric oscillatorefficiently converts the pump radiation to continuously tunable signal and idlerfrequencies.

There are a number of configurations for an optical parametric oscillator (OPO),.The first distinction is between cw and pulsed operation. Due to the much highergains, we consider only pulsed operation where the pump is typically generatedby a Q-switched laser source. Parametric oscillators have also operated internal tothe pump laser cavity, but the external configuration is more common. Finally, thereare different parametric oscillator cavity configurations. The two most importantare the doubly resonant oscillator (DRO), where both the signal and idler wavesare resonated by the cavity mirrors, and the singly resonant oscillator (SRO), whereonly one wave is resonant. The operation characteristics of parametric oscillatorswith these cavity configurations have been discussed in detail in the review articlesby Harris (79), Smith (84), and Byer (85).

The important differences between DRO and SRO operation include threshold,frequency stability, and pump laser frequency requirements. The threshold of aDRO occurs when the gain equals the product of the signal and idler losses or

F2lZ sinc2 (~1) -- = ala2 22.

where F2/2 given by Equation 19 is the single pass parametric gain and a2, a1 are thesingle pass power losses at the signal and idler. The SRO threshold is greater thanthat of the DRO. If the idler wave at ~ is not resonated, then the SRO thresholdbecomes

F212 sine2 (-~) = 2a2 23.

which is 2/al times greater than the DRO threshold. As an example consider a5 cm long 90° phasematched LiNbO3 crystal pumped by the second harmonic ofa Nd:YAG laser at 0.532/tm. The DRO pump power threshold for 2~ losses at091 and o92 is only 38 mW. The SRO threshold is increased to 3.8 W. For cw pumplasers the DRO is required in order to achieve threshold. However, for pulsedparametric oscillator operation where kilowatts of pump power is available, thehigher SRO threshold is not a disadvantage and singly resonant offers significantadvantages over doubly resonant operation.

One obvious advantage of the SRO is the much simpler mirror coating require-ment since only one wave is resonated. The DRO also requires a single frequencypump wave (79), whereas the SRO can be pumped by a multiple axial mode sourcewhich more closely approximates typical laser characteristics. Finally, the DROoperates with large frequency fluctuations since tl~e condition ~op = 09,+~01 musthold for each parametric oscillator cavity mode and pump frequency. This leads tomode jumping and the so-called "cluster effect" (67) in output frequencies where

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 165

only a cluster of a few adjacent axial modes oscillate within the gain lincwidth ofthe parametric oscillator. Since the SRO has only a singlc cavity none of thesefrequency competition effects occur. In fact, the SRO can be pumped with a multipleaxial mode pump laser source and still operate at a single frequency for theresonated wave. These factors make singly resonant operation desirable wheneverpossible.

The conversion efficiency of parametric oscillators has been studied in detail andis discussed in the previously mentioned review papers. Briefly, the DRO theoreticallyshould be 50~o eff~cient and the SRO near 100~ efficient. In practice the DROefficiency approaches 50~ and the SRO efficiency is near 40~o although 60-70~conversion efficiencies have been obtained.

The tuning and bandwidth of a parametric oscillator are determined by the

phasematching condition k3 = k2 + k1 and the sinc (Ak//2) phase synchronism factor.

2000

4000

6000

8oo0

I0,000

12,000

14,000

16,000

~8,000

ZO,O00

- 5000

~561.0

Xp = 5;’6.0:5z6.o

"~’~.....~p = 475.5

SIGNAL

200 2:50 300 :550 400TEMPERATURE eC

4000

3000

2000

1500

I000

900

800

750

7O0

650

- 600

- 550

500

450

Fi.qure 2 LiNbO3 parametric oscillator tuning curves for various doubled Nd : YAG laserpump wavelengths.

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

166 BYER

In general, a parametric oscillator is tuned by altering the crystal birefringence. Thisis usually done by crystal rotation, thus changing the extraordinary index ofrefraction, or by controlling the crystal temperature and thus the birefringence. Asan example Figure 2 shows the temperature tuning curves ofa LiNbOs parametricoscillator pumped by various doubled wavelengths of a Q-switched Nd : YAG laser.The tuning range extends from 0.55 to 3.7 #m. Tuning curves for a number of non-linear crystals have been given in the review article: by Byer (85).

The gain bandwidth of a parametric oscillator is found by analyzing thesinc2 (Ak//2) function. Letting Ak//2 = n define the bandwidth gives

~co = 2~/fll

where

~ = [(~3k~/~309~)-(¢3k2/6q¢02)]

is the crystal dispersion factor. Expanding fl in terms of the crystal index ofrefraction shows that fl ~ 2An/c so that the parametric oscillator gain bandwidthin wavenumbers is approximately

124.Ibv (cm- 1)I -- 2Ant

where An is the birefringence and l the crystal length. A 5 cm long LiNbOsparametric oscillator has approximately a 1 em- ~ gain bandwidth.

Like laser sources, the parametric oscillator can oscillate over a narrowerfrequency range than the full gain bandwidth. In this regard, the parametricoscillator acts like a homogeneously saturated laser and can operate in a singleaxial mode without a reduction of the conversion efficiency, Linewidths as narrowas 0.001 cm- 1 or 30 MHz have been achieved wifh LiNbO3 parametric oscillators(for further discussion see Byer, 85).

More than any other device the optical parametric oscillator requires a uniformhigh optical quality, low loss nonlinear crystal. In addition, the crystal must haveadequate birefringence to phasematch and be able to withstand the high laserintensities needed to reach threshold without damaging. These linear and nonlinearoptical material requirements are discussed in detail in the following section.

NONLINEAR MATERIALS

Material Requirements

Nonlinear crystals must satisfy four criteria if they are to be useful for nonlinearoptical applications. These criteria are adequate nonlinearity and optical trans-parency, proper birefringence for phasematching, and sufficient resistance to opticaldamage by intense optical irradiation. These properties are briefly discussed in thenext four sections. They are then illustrated by descriptions of useful nonlinearcrystals.

NONLINEARITY In the early days of nonlinear optics adequate laser power was notalways available to take full advantage of the potential conversion efficiency of a

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 167

nonlinear crystal. Under those circumstances, the highest crystal nonlinearity was avery important factor. Since the late 1960s the situation has changed chiefly due tothe availability of well controlled high peak power laser sources at many wave-lengths across the ultraviolet, visible, and infrared spectral regions. Under presentcircumstances, the crystal nonlinearity becomes only one factor in determining thecrystal’s potential for nonlinear applications. For example, if more than adequatelaser power is available, then the nonlinear conversion efficiency is determined bythe maximum incident intensity the crystal can withstand without damaging. Inaddition, the nonlinear conversion efficiency is then more usefully expressed at agiven intensity rather than power level. Finally, in comparing nonlinear crystals withmore than five orders of magnitude range in their figures of merit as illustratedby Figure 1, one finds that most crystals have very nearly the same conversionefficiency at a fixed intensity. This remarkable fact is illustrated by Figure 3 which

1.0

0.10

0.01

0.001

ILiNbO3 (5 cm)

ZnC~P~(I)

~ Te I ZnGeP2(Tr)I ADP (Scn

CdSe (2cm)AgGaSez

A GoS I TI3AsSe3

I AgaAsS3

LIT03

TRANSPARENCY RANGE (p.m)

Figure 3 Nonlinear conversion efficiency (parametric gain) at 1 MW/cm2 pump intensityand transparency raiage of nonlinear crystals. The pump wavelength for parametric con-version (second harmonic wavelength for SHG) is shown by the vertical tick mark. Thenonlinear efficiency varies as the square of the pump wavelength and crystal length. Thecrystal lengths are taken to be 1 cm unless specified.

20 I0 5 2 I 0.5 0.2

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

168 BYER

shows the parametric gain for a number of nonlinear materials. Under the presentcircumstances, the magnitude of a crystal’s nonlinear coefficient is not of paramountimportance, but must be taken into account along with the other material parameters.

The measurement of crystal nonlinear coefficients has continued at a rapid paceso that there are extended tables available listing nonlinear coefficients (35, 85, 95,122). The measurement of absolute nonlinear coefficients has been carried out by number of methods including second harmonic generation (140, 141), mixing (58),and parametric fluorescence (137). The latter method has the advantage of being relative power measurement and not requiring the absolute measurement of poweras for SHG. Relative nonlinear coefficient measurements have also been made bythree methods: the powder technique (142), the Maker fringe method (4, 143), the wedge technique (144-146). The latter method is particularly useful in that gives, in addition to the relative magnitude of the nonlinear coefficient, the relativesign and the coherence length of the interaction. At this time, absolute nonlinearcoefficients have been measured for a number of’ crystals including ADP, KDP,LilO3, LiNbO3, Ag3SbS3, CdSe, and AgGaSe2. In tlhe visible LilO3 and KDP and inthe infrared GaAs are used as standard nonlinear crystals. There is interest inimproving the accuracy of measurement for nonlinear coefficients and work is inprogress toward that goal.

TRANSPARENCY Known nonlinear materials have transparency ranges that extendfrom 2200 A in ADP through the infrared in a number of semiconductor compoundsand. beyond the reststrahl band into the far inti’ared in both oxide and semi-conductor crystals. In general, the transparency range in a single material is limitedby the band edge absorption at high frequencies and by two-phonon absorptionat twice the reststrahlen frequency at low frequencies. Materials are also transparentin the very low frequency range between dc and the first crystal vibrational mode.Thus nonlinear interactions may extend from the ultraviolet through the visible andinfrared to the far infrared. In fact, only a few crystals having the proper bire-fringence and overlapping transparency ranges are needed to cover the entireextended frequency range. This is important because the growth of high opticalquality nonlinear crystals is, in general, a difficult task. In addition, nonlinearcrystals that can be grown well, are transparent, and have proper birefringence forphasematching are very rare among all known acentric crystals (147). For example,among 13,000 surveyed crystals only 684, or 5.25~o, are uniaxial and phasematchable,and of these less than half have a nonlinearity greater than KDP and far fewer areamenable to crystal growth in high optical quality centimeter sizes.

The transmission loss in a nonlinear crystal reduces the SHG conversionefficiency by e-t~2/2+~1)l where ~2 and ~1 are the loss per length at the secondharmonic and fundamental waves. Thus a 0.05 cm-- ~ and 0.025 cm- ~ loss at 209 and09 in a 1 cm long crystal reduces the SHG efficiency by 0.95, which is negligible.However, in a 5 cm crystal the same losses reduce the efficiency by a factor of0.77, which is significant. High optical quality oxide materials have losses in the10- 3 to 10- 5 cm - 1 range, whereas semiconductor rnaterials show much higher lossesin the 1 cm-~ to 10-~ cm-~ range. The reduction of optical loss in nonlinear

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 169 "

crystals is important if the nonlinear interaction is to proceed efficiently. It becomeseven more important for operation of a parametric oscillator where the thresholdpumping power and operating efficiency directly depend on the crystal and cavitylosses.

Recently intensity-dependent losses have been recognized as important factors inthe transparency of a crystal. At the short wavelength end of a material’s trans-parency range, two-photon absorption may become the dominant loss mechanismeven in a frequency range that is normally transparent to low intensity radiation.For example, at 10 MW/cm2 the two-photon absorption in GaAs at 1.32 #m is0.3 cm 1, which is significant compared to the 0.05 cm-1 normal absorption loss(148). This nonlinear absorption mechanism has also been observed in oxide non-linear materials for intense pump radiation within the two-photon frequency rangeof the band edge. Thus for maximum efficiency, pump wavelengths must be longerthan the two-photon absorption edge of the nonlinear crystal, although operationnear the band edge is possible at lower efficiencies and pump intensities. Gandrud& Abrams (45) have reported an additional loss mechanism in tellurium due two-photon induced free carrier absorption. This mechanism reduced the SHGconversion efficiency from 15 to 5~o for doubling a CO2 laser source.

The two-photon absorption limit was in mind when pump wavelengths for theparametric gain calculations shown in Figure 3 were chosen. Figure 3 does illustratethat with a few nonlinear materials, nonlinear interactions are possible over theentire 2200 A to 30/~m spectral region. Thus there is the possibility of generatingcontinuously tunable coherent radiation in nonlinear crystals over this extendedspectral range.

BIREFRINGENCE AND PHASEMATCHING For efficient nonlinear interactions phase-matching must be achieved in the nonlinear crystal. As an example, SHG in cubiccrystals that lack birefringence and thus are not phasematchable occurs only overa distance of one coherence length between 10-100/~m. By using birefringence tooffset dispersion, the phasematched interaction may proceed over the full crystallength, or approximately I cm. Since the SHG efficiency varies as 12, phasematchingincreases the efficiency by at least 10’~. The enormous improvement in nonlinearconversion efficiency due to phasematching makes phasematching essential in non-linear crystals. Thus if a crystal is nonlinear and transparent, it must still phasematchto be useful. Adequate birefringence for phasematching is the most restrictiverequirement placed on a crystal and reduces the number of potential crystals to onlya few hundred out of over 13,000 known crystals.

In conducting surveys for new nonlinear crystals, the crystal symmetry is deter-mined by X-ray methods or by reference to existing tables (149). If the crystal acentric and belongs to a point group that gives nonzero nonlinear coefficients forphasematching (see Kurtz, 122, for further discussion) then the crystal indices refraction and birefringence must be determined. Fortunately, mineralogy texts anddata collections are available (150) which list indices of refraction and birefringencefor a large number of crystals. A comparison of the crystal birefringence against itsindex of refraction and similar quantities for known phasematchable crystals gives

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

170 BYER

a quick indication of whether the potential nonlinear crystal has adequate bire-fringence for phasematching. Wemple (151), Wemple & DiDomenico (152), and (147) have plotted birefringence vs index of refraction for known nonlinear crystalsto determine the minimum required birefringence for phasematching. Such plots areuseful since birefringence of a particular crystal cannot accurately be determinedtheoretically at this time.

Of course the above preliminary indications of possible phasematching in a newmaterial must be carried a step further to determine the actual phasematchingproperties of a crystal. This is usually done by accurately measuring the crystalindices of refraction and fitting the results to an analytical expression which is usefulfor phasematching calculations. The measurement of crystal indices of refraction istedious experimentally, especially in the infrared, so that complete measurementshave been made on only a few crystals (35, 95). The measurements must be accurateto 0.01~ for phasematching calculations to be made. For calculation purposes, theindex values vs wavelength are usually expressed by a Sellmeier equation ormodified Sellmeier equation. Once in this form, the phasematching expression forSHG n~ = nZe~(O) can be solved directly for the phasematching angle 0. For three-frequency phasematching conditions, a small computer program is usually written tosolve simultaneously the two equations coa = ~oz + o~a and ka = k2 + k1 where k =2~zn(2)/2. Care must be taken in solving these equations since they may be doublevalued. The LiNbO~ parametric oscillator tuning curves, shown in Figure 2, werecalculated in this manner using analytical expressions for the index of refractiongiven by Hobden & Warner (153).

Nonlinear crystals must also have a very uniform birefringence over the crystallength for efficient nonlinear conversion. Birefringence uniformity places one of themost stringent requirements on the growth of quality nonlinear crystals. Nash etal (154) have discussed the reduction in conversion efficiency due to birefringentnonuniformities.

Another limitation to nonlinear conversion efficiency is the breaking of phase-matching due to thermally induced birefringence changes. This problem has beentreated in detail for SHG by Okada & Ieiri (155). They show that the optimumphasematching temperature shifts with increasing average laser power. In crystalswith a large birefringence change with temperature, such as ADP and LiNbOa,thermal breaking of phasematching becomes serious at average power levels near1 W. On the other hand, crystals such as LiIOa which have a small temperaturevariation of birefringence can handle much higher average powers.

DAMAGE INTENSITY An important limitation to the maximum nonlinear conversioneff~ciency is crystal damage due to the input laser intensity. Laser induced damagemay be the result of a number of interactions in the material. Ready (156) discussespossible damage mechanisms in a monograph on the effects of high-power laserradiation. Among the mechanisms considered are thermal heating, induced ab-sorption due to multiphoton absorption which leads to heating or to breakdown,stimulated Brillouin scattering, self-focusing, surlhce preparation, and dielectricbreakdown. Thermal heating, in which the temperature rise of the material isproportional to the input pulse duration or deposited energy is a common damage

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 171

mechanism in metals and highly absorbing materials. Semiconductors behave morelike metals than dielectrics for this form of damage. Ready (156) lists semiconductordamage thresholds (see p. 305 of ref. 156) as energy dependent near 5-10 J/cm2. Fora 100 nsec laser pulse the damage intensity is thus 5~100 MW/cm2 which agreeswith reported values for silicon and germanium (157). For 1 nsec pulses the powerdensity increases by 100 to greater than 1 GW/cm2 if thermal damage remains thedominant mechanism. There is experimental evidence in GaAs that such high damagethresholds are reached for pulses near 1 nsec. This has important implications forinfrared nonlinear optics since, in general, parametric gains are limited by the muchlower 20-60 MW/cm2 damage threshold for long pulses. In the limit of cw pumping,semiconductor materials have damage thresholds as low as 1 kW/cm2 due to surfaceheating and melting.

Damage thresholds for dielectric materials are generally much higher than forsemiconductors. For example, sapphire damages near 25 GW/cm2 for Q-switch pulseirradiation. Glass & Guenther (158) have reviewed damage studies in dielectrics. Theypoint out that nonlinear materials show a marked decrease in damage thresholdfor phasematched second harmonic generation. For example, LilO3 shows surfacedamage at 400 MW/cmz for 10 nsec pulses. When phasematched it damages at30 MW/cm2 for the fundamental and 15 MW/cm2 for the second harmonic. Similarresults have been noted in LiNbO3 and Ba2NaNbsO15.

In a series of very careful studies, Ammann (159) measured LiNbO3 surfacedamage thresholds with various quarter wave coatings. He found that uncoatedLiNbO3 damages at 40 MW/cm

2 at 1.08 ~m for a 0.5 W, 4 kHz, 140 nsecrepetitively Q-switch laser source. The damage threshold was increased to 150MW/cm2 for a 2/4 layer ofA1203-coated LiNbO3 crystal. Additional measurementson thin ZnS films showed the importance of overcoating and the lowering of thedamage threshold with time upon exposure to air (160). Similar lowering of damagethreshold for ThF2 overcoated CdSe crystals used in an infrared parametric oscillatorhas been noted (161). In that case the damage threshold decreased from 60 MW/cm2

to 10 MW/cm2 over a period of a few days. In addition, damage occurred muchmore readily along surface scratches, indicating that surface preparation is important.

Bass & Barrett (162) proposed a probabilistic model for laser induced damagebased on an avalanche breakdown model. For this damage mechanism, the laserfield acts as an ac analog to dc dielectric breakdown. A laser power density of10 GW/cm2 corresponds to 4 x 106 V/cm, which is close to the measured dc dielectricbreakdown fields near 30 x 106 V/cm. Bass & Barrett (162) have presented the laserdamage threshold in a probabilistic way such that the probability to induce surfacedamage is proportional to exp(-K/E) where K is a constant and E is the rootmean square (rms) optical field strength. Measured dielectric breakdown intensitieslie near 25 GW/cm2 for glasses and fused silica and between 24 GW/cm2 for non-linear crystals. It appears that if other damage mechanisms to not limit the laserintensity at lower levels, then laser induced dielectric breakdown determines themaximum incident intensity. Efforts to understand the mechanisms of laser induceddamage have been increasing (163, 164). Hopefully these studies will lead to a betterunderstanding of the material’s damage intensity limits.

Fortunately the damage intensity for most useful nonlinear materials lies between

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

172 BYER

10 MW/cm2 and 1 GW/cm2. Figure 3 then shows that nonlinear conversioneflicicncies or parametric gains are high for crystal lengths on the order of 1 cm.The damage intensity does place a limit on the-energy handling capabilities ofnonlinear crystals. Thus Q-switched laser pulse ene:rgies transmitted through 1 cm2

area crystals are limited to 1-10 J. For most applications of nonlinear crystals thisis not a serious limit since the laser host medium and the nonlinear materialdamage at similar energy densities.

KDP and its Isomorphs

KDP, ADP, and their isomorphs are ferroelectric crystals (165) belonging to the742m tetragonal point group above their Curie temperatures. KDP crystals aretransparent from 0.21 to 1.4/~m for the nondeuterated and 0.21 to 1.7 /~m for thedeuterated material (166). ADP has a similar transparency range. KDP and itsisomorphs are negative birefringent and are phasematchable over most of theirtransparency range. For a complete reference to crystal indices of refraction seeMilek & Welles (166), Bechmann & Kurtz (95), and Singh (35).

Because of the availability of large, high optical quality crystals, KDP and ADPwere the subject of early nonlinear optical experi~nents by Miller et al (167) andMiller (21). Later Francois (140) and Bjorkholm & Siegman (141) made accuratecw measurements of ADP’s nonlinearity. In addition, Bjorkholm (168) has madecomparative nonlinear coefficient measurements of other crystals relative to KDPand ADP.

KDP and ADP have played a significant role as efficient second harmonicgenerators for both cw and pulsed sources. For cw doubling ADP and KDP canbe temperature tuned to the 90° phasematching condition over a limited range offundamental wavelengths between 0.54 /~m and 0A9 /~m at temperatures between+60°C and -80°C (169, 170). In particular, ADP and KDP ° phasematch fordoubling 5145 A at - 9.2°C and - 11.0°C. Other isomorphs of KDP 90° phasematchover different wavelength regions. For example, Rubidium dihydrogen arsenate(RDA) ° phasematches for doubling th e 0.694 #~n Ruby laser (171) and Cesiumdihydrogen arsenate (CDA) ° phasematches for doubling 1.06 #m(172).

Using 90° phasematched ADP, Dowley & Hodges (169) obtained up to 100 of 2573 A in 1 msec pulses and 30-50 mW of cw power. The doubling wasperformed internal to an argon ion laser cavity to take advantage of the highcirculating fields. The SHG efficiency was strongly dependent on crystal losses.

The ultraviolet transparency and phasematching characteristics of KDP isomorphcrystals make them useful for ultraviolet generation by sum and second harmonicgeneration. Huth et al (173) were the first to demonstrate this capability externally doubling a dye laser source. Similarly Yeung & Moore (174) and Sato(175) have generated tunable ultraviolet between 3()44-3272 A by summing a pumped dye laser and a Ruby laser.

Wallace (176) reported an intracavity doubled dye laser that tunes between 2610and 3150 A. This source uses a Q-switched internai[ly doubled Nd:YAG laser as apump source for the rhodamine 6G and sodium ltuorescein dye laser. The ADPintracavity doubled dye laser produced 32 mW of average power at 2900 A in a

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

NONLINEAR OPTICAL PHENOMENA AND MATERIALS 173

2 3 cm-~ bandwidth. The conversion efficiency from input doubled Nd:YAG toultraviolet power was 4.3~o. At the 65° phasematching angle used for doubling therhodamine 6G dye laser, the ADP double refraction angle is/9 = 0.025 rad, whichresults in a conversion efficiency to the second harmonic of 1~o per 100 W ofinput power.

Using a 1 J per pulse 10 pulse per second Nd:YAG laser source, Yarborough(177) has obtained high ultraviolet pulse energies and average powers. For the1.06 ~m source Yarborough uses a flashlamp pumped 1/4" diameter rod Nd : YAGoscillator followed by 1/4" diameter and 3/8" diameter rod amplifiers. This source isdoubled in a 90° phasematched CD*A crystal at 45~o efficiency yielding 450 mJ,0.532/~m pulses. The CD*A phasematches at 103°C and the incident 1.06/~m poweris unfocused into the 20 mm CD*A crystal. The green 0.532 #m source is doubledinto the ultraviolet in a 2 cm long 90° phasematched ADP crystal. The conversioneff~ciency for this step is 22~, yielding 100 mJ pulses at 0.266/~m. The harmonicgeneration in both CD*A and ADP takes place without damage to the crystals.The power levels reported are limited by the laser source becoming unpolarized athigh pumping levels. Simultaneously, thermal heating of the doubling crystals beginsto limit the second harmonic generation efficiency. The ultraviolet source has beenused as a pump for an ADP parametric oscillator (66). In addition, the greenoutput at ~).532/~m has been used to pump dye lasers with up to 60~o conversionefficiency.

The high energy, high average power source reported by Yarborough illustratesthe optical quality of KDP and its isomorphs. In addition, the use of 90° phase-matching for efficient second harmonic generation demonstrates its advantage inthese experiments. Although KDP-type crystals have not been utilized extensivelyin parametric oscillator studies, they play an important role in generating tunableultraviolet radiation by second harmonic and sum generation of tunable visibleSOUrCes.

LiNbO3 and LilO3LiNbO3 is a ferroelectric material (178) with a Curie temperature approximately40°C below its melting point of 1253°C. Since the recognition of the uniqueelectro-optical (179) and nonlinear optical (180) properties of LiNbO3 in 1964, it hasbeen extensively studied (181). The growth and physical properties of LiNbO 3 havebeen discussed in a series of papers by Nassau et al (182) and by Abrahams et (183-185). The electro-optic coefficients for LiNbO3 have been measured by number of workers (186-189), as have the indices of refraction (153, 190, 191). particularly useful form for the refractive 5ndices, including temperature dependence,is given by Hobden & Warner (153).

Early work with LiNbO3 showed two potentially troublesome optical properties:optically induced inhomogeneities in the refractive index (11, 192-196) and growth-dependent birefringent variations (197-200). The optically induced index inhomo-geneities were found to be self-annealing for crystal temperatures above approxi-mately 180°C for visible radiation and 100°C for near infrared radiation. This factled to attempts to grow "hot" LiNbO3 by adjusting the composition (198) and

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F

or p

erso

nal u

se o

nly.

http://www.annualreviews.org/aronline

174 BYER

doping with MgO to increase the birefringence to achieve phasematching for 1.06 #mat temperatures approaching 180°C. In addition, new but related crystals such asBaNaNb5015 (39, 201) were grown in an attempt to overcome the index damageproblem. Unfortunately, these attempts were not successful due to the poor crystalquality that resulted from doping LiNbO3 and to the striations inherent inBa2NaNb5015 crystals.

Although growth striations severely limit the size and quality of BaaNaNb5015crystals, they have been used to double cw Nd:YAG lasers (39, 202) with goodefficiency. The nonlinear coefficient, which is approximately three times that ofLiNbOs, partially offsets the disadvantage of smaller crystals of less optical quality.Serious attempts to grow striation-free Ba2NaNb5Ol~ crystals have not beensuccessful so that the use of this material is not widespread.

The growth-dependent birefringent variations in LiNb.Oa were less difficult toeliminate. The problem was solved by growth of LiNbO3 from its congruent meltingcomposition near a lithium to niobium ratio of 0.48 mole ~o (203-205). The growthof LiNbO3 crystals from a congruent melt plus improved optical quality tests (199,206) led to uniform high quality single crystals of over 5 cm in length.

Ferroelectric LiNbO3 has a large variation of birefringence with temperature.This allows SHG at 90° phasematching for fundamental wavelengths between 1 and3.8 #m at tcmpcratures between 0°C and 550°C. Conversely, LiNbO3 90

° phase-matches for parametric oscillation for a number of pump wavelengths and can betemperature tuned over a broad spectral region. Figure 2 shows the parametricoscillator tuning curves for various pump waveleng~ths of an internally doubled Q-switched Nd : YAG laser. These LiNbOs phasematching curves were calculated byusing the Hobden & Warner (153) index of refi-action expressions. AdditionalLiNbO3 tuning curves, including angular dependence, are given by Harris (79, 207)and Ammann et al (208).

The internally doubled Q-switched Nd:YAG pumped LiNbO3 parametricoscillator is the best developed parametric oscillator at this time. This system isdescribed by Wallace (209). The Nd:YAG laser pump source operates with internal LilO3 doubling crystal, acousto-optic Q-switch, and two Brewster angleprisms for wavelength selection. The combination of four doubled Nd: YAG pumpwavelengths and temperature tuning allows the oscillator to cover the 0.54 to

Table 1 LiNbO3 parametric oscillator operating pararneters

Average Pulse Laser PumpTuning Range Peak Power Power Length Wavelength

(/~m) (W) (mW) (nsec) (/~m)

3.50-2.50 80-150 5-10 70 0.5320.975-2.50 250-350 30 80 0.6590.725-0.975 250 20 200 0.5620.623-0.760 250 50 150 0.5320.546-0.593 300 3-5 200 0.473

www.annualreviews.org/aronlineAnnual Reviews

Ann

u. R

ev. M

ater

. Sci

. 197

4.4:

147-

190.

Dow

nloa

ded

from

arj

ourn

als.

annu

alre

view

s.or

gby

Sta

nfor

d U

nive

rsity

Rob

ert C

row

n L

aw L

ib. o

n 12

/21/

06. F